research papers
The interpretation of polycrystalline coherent inelastic neutron scattering from aluminium
^{a}Physics and Materials Research Centre, University of Salford, The Crescent, Salford, Greater Manchester M5 4WT, United Kingdom, ^{b}Nanochemistry Research Institute, Department of Chemistry, Curtin University, PO Box U1987, Perth, Western Australia WA6845, Australia, and ^{c}ISIS Facility, STFC Rutherford Appleton Laboratory, Chilton, Didcot, Oxfordshire OX11 0QX, United Kingdom
^{*}Correspondence email: d.roach@salford.ac.uk
A new approach to the interpretation and analysis of coherent inelastic neutron scattering from polycrystals (polyCINS) is presented. This article describes a simulation of the onephonon coherent Q, ω) regions where onephonon scattering is allowed. These features may be identified with the same features apparent in the measured total coherent inelastic cross section, the other components of which (multiphonon or multiple scattering) show no sharp features. The parameters of the model can then be relaxed to improve the fit between model and experiment. This method is of particular interest where no single crystals are available. To test the approach, the polyCINS has been measured for polycrystalline aluminium using the MARI spectrometer (ISIS), because both dynamical models and measured dispersion curves are available for this material. The models used include a simple LennardJones model fitted to the elastic constants of this material plus a number of embedded atom method force fields. The agreement obtained suggests that the method demonstrated should be effective in developing models for other materials where singlecrystal dispersion curves are not available.
from a model of an arbitrary The onephonon component is characterized by sharp features, determined, for example, by boundaries of the (1. Introduction
Traditionally, inelastic neutron scattering measurements have involved either incoherent inelastic neutron scattering from polycrystals or coherent ). Since this time, software development and advances in computing power have made it possible (though still demanding) to generate models and to fit them to the data.
(CINS) from single crystals. The reason that CINS from polycrystals has not been employed to a significant extent in the past is that the process of integrating the scattering intensity over crystallite orientations tends to obscure the useful information that is easily available from the direct measurement of dispersion curves for single crystals measured using a tripleaxis spectrometer. However, many important materials can only be obtained in polycrystalline forms, and hence it is of interest to investigate ways of interpreting the coherent from such samples. One early attempt to do this using coherent from was made by one of the authors (Ross, 1973There are already several software packages able to calculate the key quantity required in neutron scattering, namely the dynamic S(Q, ω), using the onephonon eigenvectors as determined via density functional theory (DFT) or other methods. Notable examples are the PHONON (http://wolf.ifj.edu.pl/phonon/) and McStas (Lefmann & Nielsen, 1999) packages, and efforts have been made to broaden the selection of scattering kernels to include calculated spectral contributions from multiplephonon scattering, multiple scattering and instrument resolution functions (Willendrup et al., 2004; DANSE project, http://wiki.danse.us) to facilitate direct comparison with the measured data. However, these `whole spectrum' methods have significant limitations. The computational expense associated with the calculation of the eigenvectors of a system is an order N^{3} problem, where N is the number of atoms in a basis set describing the as the number of atoms in a system increases, so the system rapidly becomes too large for the application of ab initio methods for the determination of the dynamical matrix. This is further compounded by the sampling requirements for a given model; as the size of the basis set of atoms used to describe the system increases, so the sampling requirements (in terms of k points sampled in reciprocal space) also increases. These two factors alone represent an effective limit to the size of the system for which S(Q, ω) may be modelled using these ab initio methods.
In the present work we focus on the calculation of polycrystalline coherent inelastic neutron scattering (polyCINS) onephonon cross sections using interatomic potentialbased methods, as these are relatively computationally efficient and are widely applicable to many systems (including those with large unit cells) and as the forceconstant parameters involved provide a convenient starting point for leastsquares optimization of the starting values. Specifically, the method has been implemented within the program GULP (Gale & Rohl, 2003), designed for dynamical calculations based on force field descriptions, via a new module known as Scatter. However, the approach described could equally well be used in conjunction with DFT packages such as CASTEP (Clark et al., 2005) or SIESTA (SanchezPortal et al., 1995), from which phonon eigenvectors may be generated.
The present method differs from a `whole spectrum' approach in that it concerns itself with the identification of prominent onephonon scattering features appearing in experimental neutron scattering from polycrystals; other contributions (multiphonon, multiple scattering, resolution broadening) would have to be included in the theoretical neutron spectra to provide a full intensity profile for matching to experimental data on a point by point basis. Onephonon processes showing sharp coherent scattering features dominate in the lowQ region of (Q, ω) space and can be observed experimentally with the best experimental resolution.
An outline of the Scatter code has already been published (Roach et al., 2007), but the methodology behind its application to the interpretation and analysis of polyCINS is new to this work. It is tested here for the rather simple aluminium system.
The structure of this article is as follows. In §2, the theory and methodology of coherent inelastic neutron scattering are described, along with details of the current implementation and the methodology associated with the identification and interpretation of onephonon scattering features. Also introduced here are four semiempirical dynamical models of aluminium that are used to compute the dispersion curves and bulk properties for each model. In §3, the present experimental measurement using the MARI spectrometer is described. In §4, the method developed for the systematic analysis of polyCINS data is used to compare our experimental data for polycrystalline aluminium with the predictions of the best of the models. The models are also compared with the singlecrystal dispersion curve data. Finally, in §5, the general applicability of the method to different materials is discussed.
2. Methodology
2.1. Background theory
The neutron scattering amplitude of a nucleus can have a number of different values, owing to neutron spin and to isotope effects, so the scattering has to be divided into two parts: coherent and ), the resulting cross section can be expressed in terms of the corresponding scattering functions, S_{coh}(Q, ω) and S_{inc}(Q, ω) for the coherent and cases, respectively. These functions, which depend only on the interactions between the nuclei, define the corresponding double differential scattering cross sections (for materials containing only one element) as follows (Squires, 1978):
The coherent part, depending on the average value of the scattering amplitude, contains all the information about the relative position and motion of the nuclei taken in pairs, while the depends only on the motions of each atom taken independently. As shown by Van Hove (1954and
Here, σ_{coh} and σ_{inc} represent the two total cross sections, Q is the momentum transfer vector [Q = (4π/λ)sinθ being the magnitude of the vector, where θ is half the scattering angle and λ is the wavelength of the incident neutrons], E′ is the of a given scattered neutron where the incident energy is E, is the average (and is the meansquare average) of the bound scattering length for the nucleus, k and k′ are the incident and final wavenumbers, respectively, of the scattered neutron, and ω is the frequency of an excited phonon. The scattering functions, S_{coh}(Q, ω) and S_{inc}(Q, ω), were originally defined as here for a single species of nucleus. However, for a general nonBravais (with unit cells containing more than one atom), the terms have to be summed over the atoms in the although this results in a scattering function which, in the strictest sense, is not S(Q, ω) as originally defined. Hence, the effective onephonon scattering functions for a system with multiple atomic species, as used here, should be written as S′_{coh/inc}(Q, ω), where
and
for neutron energy gain [ and 〈n_{s}〉] and energy loss [ and 〈n_{s} + 1〉] of a system, generating a phonon of wavevector q. Here n_{s} is the number of phonons in mode s at thermal equilibrium. In equations (3) and (4), N is the number of atoms in the in the (nonBravais) system and the inner summation is over these atoms, d, with mass M_{d} and a position vector within the of r_{d}, while W_{d} is the associated Debye–Waller factor. The outer summations are over τ, the vector, and s, the phonon mode of frequency ω_{s}, providing a polarization vector e_{ds} for each normal mode, as obtained by solving the dynamical matrix. The reader should be aware that some texts adopt slightly different definitions of the phase factor of the polarization vector. For example, the text by Turchin (1965) defines the phonon wave at a position r_{d} within the to have the phase of the travelling wave at that point, whereas Squires (1978) defines this wave as having a phase relative to that of the travelling wave at the corner of the The Turchin version leads to a different general formulation of the coherent inelastic cross section from that given in equation (3). This `frame of reference' difference, whilst being irrelevant for a monatomic is crucial to the present objective for the case of more than one atom/unit cell. Here the form of the polarization vector used by Turchin will be adopted, as this is the form employed in GULP. Hence the corrected form of equation (3) is
where ξ_{ds} is the polarization vector on the alternative definition given above.
Once the expressions for the neutron scattering functions have been established, the next step is to introduce the means by which the phonon frequency (square root of the eigenvalue) and the polarization vectors (eigenvectors) are obtained for a given phonon wavevector, q. The approach, briefly summarized here, follows the standard Born–von Karman method (Born & Huang, 1956), where forces are described in terms of potentials between pairs of atoms. This method results in the construction of a dynamical matrix of the form
for each of the pairwise vectors, r, at wavevector, q. The eigenvalues, ω(q), and eigenvectors, ξ, are then obtained from equation (7):
which is solved using (I is the identity matrix) and hence by diagonalizing the resultant matrix. For every q vector there is thus a set of 3d eigenvalues (and therefore frequencies) and for each eigenvalue a corresponding eigenvector (i.e. a set of polarization vectors) for each of the d atoms; this results in the notation ξ_{ds} and ω_{s} for eigenvectors and eigenvalues, respectively.
The frequencies and polarization vectors so obtained are then used to calculate the scattering function presented in equation (5). When performing a powderaveraged calculation, it is necessary to sample in a series of concentric shells, each corresponding to a given magnitude of the momentum transfer vector, Q, as it is rotated through θ and φ. For each magnitude and orientation of Q, the program calculates the corresponding values of q by selecting the nearest point and taking q relative to this point. From this value of q, the dynamical matrix [equation (6)] is then generated and the corresponding eigenvalues and eigenvectors obtained [see equation (7)]. Fig. 1 illustrates this sampling method, along with a diagrammatic representation of the Q vector relationship with the vector, τ, and phonon wavevector, q.
The resulting data are then output using a histogramaveraging method, where defined intervals are used to create a Q (referred to as Q, where Q = Q) and to a set frequency interval. The intensities obtained for this interval in Q are sorted into the specified histogram in ω. Assembling such slices for each Q yields S(Q, ω). Resolution broadening of the scattering δ functions in Q and ω, Debye–Waller factors may be applied before summation of the intensities, but this is not necessary for present purposes.
of data `pixels'; here each pixel corresponds to a set range in the amplitude of2.2. Semiempirical force constant modelling of aluminium
Aluminium is a very well studied material that has attracted attention of late owing to the interest in the use of light metal hydrides for hydrogen storage (Schuth et al., 2004; Kang et al., 2004). Results from recent work (Budi et al., 2009) on the generation of new semiempirical force constant models for use in cluster calculations has typically been compared against reliable DFT calculations (Pham et al., 2011) (where comparisons are normally made with zone boundary frequencies), bulk properties (as above), and the density of vibrational states as obtained by both measurement and calculation (Tang et al., 2010). The simplicity of its and the proliferation of these fitting models suggest the use of aluminium as an ideal test material for the methodology presented.
When selecting models for aluminium from the large number of possible variants in the literature the emphasis here has been to test the utility of models in frequent use. For convenience, we will start with a simple LennardJones 12–6 potential (LennardJones & Ingham, 1925) fitted to the elastic constants (C11, C22 and C44) of aluminium, following the approach suggested by Halicioǧlu & Pound (1975). Although this type of model is generally considered unsuitable for the study of metallic systems, its very unsuitability (as well as its very low computational cost and the rather general nature of the potential itself) suggested its use as a model for assessing the more heavily parameterized (and considerably more computationally expensive) embedded atom method potentials.
The most successful methodology applied to the semiempirical modelling of metals, however, is the embedded atom method (EAM) (Daw & Baskes, 1983), originally developed by Daw and Baskes to study hydrogen embrittlement in nickel and now adapted for use in dynamics and cluster calculations. For this reason, it was decided to test the effectiveness of potentials of this type for predicting the dynamical properties of aluminium and to compare the results with the simplest available potential – the LennardJones (LJ) model, described above.
The EAM models most frequently used in studies of pure and alloyed periodic systems are the Sutton–Chen functional EAM potential (Sutton & Chen, 1990), the Cleri–Rosato tight binding EAM potential (Cleri & Rosato, 1993), the Streitz–Mintmire EAM potential (Streitz & Mintmire, 1994), the Mei–Davenport modified EAM (MEAM) potential (Mei & Davenport, 1992) and the parameterized EAM (NPB; Jasper et al., 2005) potential. Sheng et al. have published results for an optimized EAM potential (Sheng et al., 2011), but as they neglected to include EAM parameters for their model (obtained by fitting to DFT calculations), it has not been practical to include this model in the comparison. Likewise the manybody potential of Mishin et al. (1999), derived from a spline fit to DFT calculations and to bulk data, provided excellent agreement with the measured dispersion curves, but the paper did not include an explicit model parameterization and so this model has also been omitted. Both the Cleri–Rosato and Streitz–Mintmire models were considered for implementation in this study, but as the emphasis here is on the analysis, these models were neglected for brevity. Hence the three models selected for further analysis are the Sutton–Chen, the Mei–Davenport and the NPB. Functional forms and explanations of these standard potentials have been omitted from the text, but the expressions and parameters used are given in Table 1.

2.3. Dispersion curves from the semiempirical models
The experimental data presented in this analysis of dispersion curve predictions are taken from the tripleaxis neutron spectroscopy study of Stedman & Nilsson (1966), as presented in Fig. 2.
As a general preamble, it is worth pointing out the salient features of what is a very well studied system. In the experimental data, the facecentred cubic (f.c.c.) aluminium structure gives rise to the expected form of the dispersion curves in the [100] and [111] directions – doubly degenerate transverse acoustic (TA) modes (as a result of the fourfold and threefold rotational symmetry along these respective axes) and a single longitudinal acoustic (LA) mode. These modes are dominated by the first nearest neighbour interaction (hence the nearsinusoidal form). Thus reasonable agreement for the gradient of the nearlinear part of the curve at low q (the velocity of sound) and the frequency at which the curves cross the zone boundary is sufficient to match the shape of the curves. The observed flattening of the [111] TA curve near the zone boundary is a consequence of contributions to bonding from electron screening and exchange interactions at the Fermi surface (Hafner & Schmuck, 1974) and, in consequence, cannot be modelled with shortranged pair potentials. However, the contribution of this feature to the dynamics (and hence to the prediction of bulk properties) is relatively small, and further consideration of this region can be neglected in the present work – especially as it can be modelled with longerrange pairwise interactions or directly via DFT.
The dispersion curves in the [110] direction, along which there is only twofold rotational symmetry, produce an LA mode and two distinct TA modes. The shapes of the TA modes are determined by the second nearest neighbour contributions (even in models that do not explicitly include this interaction); the maximum for the higherfrequency TA mode (found to be displaced from a symmetry point) is determined by the second nearest neighbour contribution, and its accurate positioning requires a model with considerably more near neighbour interactions (eight to ten interaction shells is typical). In aluminium, this maximum is found close to (0).
Turning to the predicted dispersion curves, the LennardJones 12–6 potential, fitted to the elastic constants, performs better than all of the EAM potentials in comparison with experiment. It should be noted, however, that this model is specifically targeted at describing the curvature of the experimental (singlecrystal) dispersion curves but is not fitted to give zero stress at this geometry. As can be seen in Fig. 2, it provides excellent agreement with the LA modes in all crystallographic directions. The lack of nearest neighbour interaction terms beyond the first predictably generates only reasonable agreement with the TA modes in the [100] and [110] directions; this clearly demonstrates the need for additional terms for second and further nearest neighbour interactions, as does the inaccurate q positioning of the [110] TA maximum, although the model does predict the maximum frequency of this mode very well.
It should be noted that the dispersion curves obtained from the EAM models, also shown in Fig. 2, were not originally compared with the experimental dispersion curve data as their main use has been for studying clusters and associated energetics. Hence, the accurate prediction of the dynamics was less relevant and poor fits are not unexpected. The Sutton–Chen model provides the worst agreement with the experimental dispersion curves, being significantly different from experiment across the entire range of q, for all three highsymmetry directions, and the prediction of the frequencies at the zone boundaries, most notably the gamma point, provides a poor dynamical description of the aluminium lattice.
The NPB model, which clearly overestimates the stiffness of the bonding between atoms, produces dispersion curves that are an improvement on those of the Sutton–Chen potential, although the overbinding of the potential produces frequencies for all modes that are considerably higher than the experimental values.
The Mei–Davenport model performs best out of the EAM potentials chosen for this comparison. This model provides a nearperfect agreement for the TA mode in the [100] direction, over the entire range of q, and gives very reasonable agreement for the LA mode in the same direction, with close agreement in the lowerq region (q < 0.5) and reasonable agreement at the zone boundary (within 20%). The [110] and [111] directions give rise to similarly reasonable agreement to that provided by the LA mode in the [100] direction: going from very good agreement at low q (q < 0.5) to reasonable agreement at the zone boundary in both highsymmetry directions (certainly superior to the other EAM potentials).
There are clearly many more subtleties in the analysis of these dispersion curves. However, the present work seeks to present the equivalency of approach between singlecrystal and polycrystalline neutron scattering, and hence further discussion is not relevant to the present objective.
2.4. Interpretation of onephonon polycrystalline coherent S(Q, ω)
The present approach assumes that the onephonon coherent scattering process is dominant in the studied system at low Q; for the aluminium system this is a reasonable assumption given that aluminium is a strongly coherent scatterer [with a coherent cross section of 1.495 b (1 b = 100 fm^{2}), contrasting significantly with the incoherent cross section of 0.0082 b]. The approach also assumes no of crystallites in the sample, as it uses spherical polycrystalline averaging (although intensity changes due to are readily introduced by altering the sampling method): again a reasonable assumption for a polycrystalline cubic system such as aluminium. The resulting contour plot of the polyCINS intensity for the fitted LJ 12–6 potential is shown in Fig. 3, which was obtained using the Scatter subroutine in the GULP program as described above. This polyCINS plot is a 300 (in Q) × 300 (in frequency or E_{T}) bin data set with 300 angular steps in θ and φ, for ranges of 0.0 ≤ Q ≤ 10.0 Å^{−1} and 0 ≤ ω ≤ 350 cm^{−1} (0 ≤ E_{T} ≤ 43.4 meV). This produces a sampling of 27 million q points and samples (Q, ω) space in an approximately equivalent Q and resolution to that provided by timeofflight instruments such as MARI. The pattern is clearly complex but can be analysed if approached systematically in the light of the experimental or calculated dispersion curves.
Fig. 4(a) shows the dispersion surface for the first mode (in this case, the longitudinal acoustic mode) overlaid with a colour map that shows the S(Q, ω) intensity for the plane (hk0) over the range of the calculation. Fig. 4(b) takes this projection and rotates it so that the (h00) dispersion surface is visible (equivalent to the allowed scattering from the longitudinal mode in the [200] direction), so that the coherence condition is illustrated; from here, one can clearly see the regions of allowed scattering [with the colour map providing S(Q, ω) intensity information – white effectively denotes regions of (Q, ω) space where there is no allowed scattering]. From Fig. 4(b), one can clearly see the regions of intense scattering around the boundaries, as well as the increased intensity corresponding to the 1/ω term in equation (5). Fig. 4(c) shows the same data, as seen from `above', viewing the (hk0) plane; this figure rather clearly illustrates the periodic boundary conditions and provides a reference point for Fig. 4(d). The white line denotes the vector from the (000) point in the out to the (420) point.
Fig. 4(d) provides an illustration of how it is that some of the sharp features are associated with vectors to more remote points. The diagram shows the (hk0) plane in and for a particular value of ω that cuts the LA dispersion surfaces close to each `allowed' f.c.c. reflection, out as far as (420). Thus the small circles represent the q vectors corresponding to the LA phonons at that value of ω. Because of the coherence condition, the sphere in Q, which has to be integrated over direction to yield the intensity expected in the polycrystalline case, has to lie in the range defined by τ − q(ω) < Q < τ + q(ω). Thus we expect to find sharp features for this value of ω where the Q sphere touches one of the small circles as illustrated, and this turns out to be along the vectors from the origin to the higher points. Noting this, and taking into account the polarization term in the intensity e_{ds}·Q, the edge features in the scattering will be pronounced for LA modes because here the phonon displacement vector is parallel to Q. Transverse modes, on the other hand, will tend to peak where the Q sphere passes through the point, as here the displacement vector is parallel to the Q vector at the point where the sphere crosses the dispersion surface at right angles (and also passes through the point). Because the steps in intensity generally occur along the [hkl] directions, they are relatively easy to identify in the integrated onephonon cross section.
The process presented here is a simple one; S′(Q, ω) – namely the LennardJones 12–6 model introduced in §4. These lines are used to calculate S′(Q, ω) going through the different (hkl) points. As expected, the cross section shows a sharp intensity step where the two spheres touch tangentially (in the longitudinal case) or peak at the (hkl) point (transverse case). This provides an initial qualitative appreciation of the features found in the polyCINS data (as discussed in §3). Further clarification, in the form of figures demonstrating this curve projection and overlay process, is provided in the supplementary text^{1} (Fig. S5).
vectors from the origin of the to the first 11 points are calculated for the model used in the theoretical generation ofThe next step in this process is to take cuts through the calculated polycrystalline S(Q, ω) data for given ω intervals integrated over a narrow band of Q values and to associate, where possible, distinct scattering features with individual dispersion surfaces in the symmetry directions selected. In Fig. 5, cuts of constant Q (having a single `bin' width of 0.0334 Å^{−1}) have been taken through the theoretical data presented in Fig. 3. Each cut, which is representative of the Q resolution available from a typical highresolution chopper spectrometer, is then inspected and the most prominent features are compared with the equivalent projections of the dispersion curves. It is observed that the steps in intensity at a given Q tend to occur where this cut crosses one of the set of `dispersion' curves calculated along higherorder τ directions, as explained above. As noted above, the intensity features observed can be classified in terms of either peaks or coherence edge features; both sets of features are determined by the structure and vibrational characteristics of the material and are governed by equation (4). For the purposes of this work, it is unnecessary to identify every feature in a given cut through the polyCINS data set, because clearly some will arise where the Q sphere touches the dispersion curve away from any symmetry direction.
In this work, coherence edge features have generally been selected for identification, as the use of experimental data requires the summation of adjacent Q bins to reduce the statistical error in the measured intensity (owing to the relatively low count rate for a given set of detectors). This results in a `smearing' of both types of sharp feature such that the peak–coherence edge paired features are often the only readily identifiable feature in a given cut through an experimental set. Therein lies the compromise implicit in this approach to the analysis of polyCINS data; a narrower range of Q over which a summation is taken results in sharper Qdependent features, but this in turn reduces the number of measured neutron counts and hence the statistical accuracy of the data. In the extreme, a full summation over the entire range of Q sampled by an instrument results in the effective application of the incoherent approximation; here all Q dependence is lost and the data collection is reduced to a phonon measurement, whereas a fine cut (as for a single detector), providing the best Q resolution, would result in excessively long measurement times to gain sufficient statistics to make an effective comparison with a model. Examples of coherence edge features in Fig. 4 include the features containing the [111] LA modes at Q = 1.0 Å^{−1} and Q = 3.4 Å^{−1} and the [200] TA coherence edge at Q = 1.8 Å^{−1}, for energy transfers of 33.8 meV (273 cm^{−1}), 29.8 meV (240 cm^{−1}) and 38.6 meV (311 cm^{−1}), respectively.
It should be noted that the full intensity of S_{coh}′(Q, ω) at a given (Q, ω) value is not exclusively the result of a single mode in a set direction in Clearly, a large number of q values contribute to a given S_{coh}(Q, ω) intensity after averaging over Q directions. However, it does seem that many of the sharp features in the scattering functions do arise from the tangential intersection of the sphere in Q with a particular dispersion curve.
2.5. Bulk properties
Here we present the bulk properties calculated from the models described in the previous section. The values are given in Table 2, along with experimental values from the literature. Note that the bulk moduli calculated with GULP use the Voigt volume derivative approach (Nye, 1957).

As shown in Table 2, the potentials all perform adequately when compared with experiment; the single exception to this is the binding energy predicted by the LJ 12–6 pair potential. As is to be expected, this twoparameter LJ model is unable to fit the binding energy, parameter and mechanical properties simultaneously. Because of its pairwise nature, the LJ 12–6 potential cannot capture the Cauchy violation between the elastic constants C_{12} and C_{44}, unlike the EAM models. However, this simple model, when fitted to the elastic constants, provides good agreement across a range of other bulk properties, in particular, the bulk moduli; the model predicts Young's modulus especially well compared with the other models. It also performs adequately for the bulk and shear moduli, although both the NPB and Sutton–Chen potentials do better, with the Mei–Davenport outperforming the LennardJones by a considerable margin. However, the LennardJones model performs very well in the prediction of Poisson's ratio; the EAM models all predict values that are significantly different from experiment. No particular conclusions should be drawn from the agreement with elastic constants as these were used to parameterize the model. Thus, on the whole, the simple LJ 12–6 model performs remarkably well with respect to the curvature of the surface; the Mei–Davenport model generally matches, or slightly exceeds, its performance for most of the bulk properties compared here, while the Sutton–Chen and NPB potentials generally have a worse overall performance in this regard.
When comparing the potential models it is important to consider the relative computational expense, given that calculations of polyCINS will require many secondderivative evaluations. As an example, the LJ 12–6 model completes a standard sampling of (Q, ω) space, as described in §2.4, about 300 times faster than the equivalent EAM calculations. To be precise, the LJ 12–6 model takes around 150 s on a 8core, 3 GHz Xeon workstation, whereas the EAM potentials average around 45 000 s on the same workstation for the identical sampling and phonon calculations; it is thus clear that the LJ 12–6 model can be useful as a tool for generating the bulk properties in systems with large numbers of atoms in the although its poor binding energy and more limited transferability to other environments, such as cluster calculations, limit its broader utility.
3. Experimental
In order to collect data across a full range of momentum and energy transfers for aluminium (necessary to investigate the Q dependence of the vibrational modes in a polyCINS experiment), the most appropriate instrument type is a direct geometry timeofflight chopper spectrometer. This type of instrument [of which the MARI spectrometer (Taylor et al., 1991) situated at the ISIS facility, UK, is a distinguished example] is designed to sample (Q, ω) space by means of a fixed incident neutron energy, where the scattered neutrons are measured using a large detector bank so that energy and momentum transfer can be recorded independently.
Data were gathered on this spectrometer over a period of 22 h, using the proton current convention for a total proton current on target of 3600 µA h for ISIS TS1. The sample was a 94 g polycrystalline sample of 99.999% purity aluminium in pellet form (manufactured by Goodfellow Cambridge Ltd) at a temperature of 10 K. The fixed incident energy was 58.8 meV, which provided a sampling of (Q, ω) space for 0 ≤ Q ≤ 10.0 Å^{−1} and 0 ≤ ω ≤ 350 cm ^{−1} (0 ≤ E_{T} ≤ 43.4 meV) in the characteristic `bishop's mitre' configuration obtained from the detector coverage in neutron energy loss. Although the instrument also collects data in neutron energy gain, neutron energy loss was preferred (and the experiment was performed at low temperatures). This approach more fully samples the region of (Q, ω) space of interest, because neutron energy gain is limited to energy transfers ∼kT, i.e. a few meV at low temperature, where there will be little intensity for energy gain above this. The data have been corrected for detector efficiency, and all other preprocessing and data reduction from raw timeofflight data to S′(Q, ω) were accomplished using the MANTID suite of neutron scattering instrumentation software (http://download.mantidproject.org/). The resulting data set is shown, with a 10% maximum intensity cutoff applied to avoid domination of the contour plot by the elastic line, in Fig. 6.
Applying the neutron scattering theory described in the previous section, it is possible to gain a good understanding of the sharp features present in such data sets owing to onephonon scattering – generally due to the sphere in Q touching and crossing particular dispersion surfaces. Multiplephonon terms, which will dominate at larger energy and momentum transfers, are considerably smoothed relative to the onephonon terms, as are multiplescattering effects.
Common to all such coherent polycrystalline S_{coh}′(Q, ω) plots, the onephonon scattering functions as given by equation (5) (as a function of Q) yield scattering intensities that, on average, increase as a function of ∼Q^{2} until attenuated by the increasing contribution of the Debye–Waller factor, exp(−W_{d}) at higher Q.
Upon visual inspection, the first and most obvious features of the data in Fig. 6 are the `arches' of very intense scattering associated with the LA dispersion curves, corresponding to the superposition of the single crystallographic directions consistent with the dispersion curves of a single crystal. These features, which dominate the scattering intensities in the experimental data, arise from the fact that, for a particular ℏω, the coherence condition implies that τ − q(ω) < Q < τ + q(ω), where q is taken along the phonon branches in highsymmetry directions in the (in particular, for aluminium, the [200], [220] and [111] directions). As seen on closer inspection, the lowersymmetry directions defined by vectors from the origin to higherorder Bragg peaks are also significant. Otherwise, given the relative complexity of these data, identifying which feature belongs to a given vibrational mode is challenging, especially when one considers systems with more than one atom per or materials with noncubic symmetry. However, it is clear that many of the dominant features in a given polyCINS data set, and, in particular, the simplest case of a facecentred cubic metal with a single elemental basis, such as aluminium, are those defined by the modes in the major crystallographic directions defined by the τ vectors of the projected out into Q. This observation informs much of the analysis provided in §4, as the approach taken to the analysis of the data relies upon the identification of scattering features using projections of dispersion curves onto momentum transfer, Q. Thus, the `arches', corresponding to the LA modes in the [111], [200] and [220] crystallographic directions as they return to the elastic line (zero energy transfer) at 2.68, 3.1 and 4.4 Å^{−1} are clearly visible, with further multiples of these at 6.2, 8.8 and 5.34 Å^{−1} and so on. These features are accompanied by the modes returning to zero obtained from the vectors to the higher points for the f.c.c. such as the [311], [331], [420], [422], [511], [531], [442] and [620] directions in the conventional (Cartesian) directions.
The other key features that are clearly identifiable from this dispersion curve comparison are the maximum energies of the LA and TA modes that give rise to cutoff features in the polyCINS scattering associated with abrupt intensity changes that are invariant in Q but seen as `bands' of intense scattering over the range of Beginning at low Q, the first such features are those due to the maxima of the LA modes of the [111] and [100] dispersion curves at Q = 1.34 Å^{−1} and Q = 1.56 Å^{−1}, respectively, at vibrational frequencies (energy transfers) of 325 cm^{−1} (40.3 meV) and 322 cm^{−1} (39.9 meV) that give rise to the highfrequency limit of the scattering. (Note that if Q is parallel to q, as in the first zone, the condition leads to the longitudinal modes having maximum intensity and the transverse modes zero intensity.)
4. Analysis of coherent inelastic neutron scattering from polycrystalline aluminium
In this section, the methodology presented in §2.4 is applied to the specific task of identifying and exploiting the polyCINS data from polycrystalline aluminium. Given that data sets obtained from powder samples can be thought of as a multitude of dispersion curves [deriving from every possible direction in (Q, ω) space] superimposed upon each other, great care should be taken in identifying any given feature as belonging to a particular phonon branch. This is particularly so, given that it was found that many of the most intense sharp features in the polyCINS data set arise where the sphere in Q crosses the dispersion surface in nonsymmetry directions. However, by extending the analysis to include crystallographic directions in other than the highest symmetry directions, many of these features can be identified. This then allows the experimentalist to identify specific features and use the frequencies of these features in a fitting process to generate theoretical models that match these features. Given that the intensities of polyCINS features are directly related to the eigenvectors for the motions of planes of atoms, this method presents an excellent means of generating physically useful models that can predict bulk properties well.
The approach taken in this work has been to identify the dominant features of the aluminium S′(Q, ω) spectrum using the simple LJ 12–6 model. Once the general features of the plots are identified, it becomes relatively straightforward to extract effective dispersive feature information in terms of more traditional dispersion curves, which can then be used to create a set of k points for use in a fitting process, as described in §4.1. This method is applied to the experimental data set to illustrate the utility and limitations associated with the analysis of experimentally obtained data. In §4.2, the same approach is applied to a comparison of the `best' of the MEAM models, the Mei–Davenport model, with the theoretical neutron spectra; dispersion curves and bulk properties are then recalculated for both models fitted to experimental data. It should be noted that no resolution correction has been added to the theoretical data, as this makes it easier to identify the coherence edges, which are then linked to the sloping edge features in the experimental data (see §4.1).
4.1. Comparison of experimental Al polyCINS S′(Q, ω) data with model predictions
As noted above, the full intensity of S_{coh}′(Q, ω) at a given (Q, ω) value is a superposition of the scattering seen in all directions. That is why it is necessary to concentrate on the identification of particular sharp features for the comparison of experiment and theory. Once S_{coh}′(Q, ω) features are identified as being associated with a given cut in the next step is to approach the experimental S(Q, ω) data and attempt to identify equivalent features. In order to facilitate the comparison, both experimental and theoretical cuts (the LJ model) through the data sets at fixed Q values may be superimposed as in Fig. 7.
We note here that there are gaps in the detector coverage on the instrument and these affect the choice of constant Q cuts. Hence a new set of cuts, chosen to pass through the sharpest, most intense onephonon features with a minimum of gaps due to missing detectors, were selected: cuts were made through both theoretical and experimental data sets for a bin width of 0.0667 Å^{−1} (median value ±0.03335 Å^{−1}) for median values of Q of 2.2, 2.5, 3.2, 3.6, 4.2, 4.6, 5.0, 5.6, 6.2, 6.6 and 7.0 Å^{−1}. The resulting comparisons are shown in Fig. 7.
Although there are significant differences in both the intensity profiles and the positions of sharp features on the S_{coh}′(Q, ω) profile is in reasonable agreement: sufficiently so to relate features in the theoretical and experimental profiles.
scale, the generalFrom these comparisons, 31 S_{coh}′(Q, ω) features could be reasonably assigned to one of the 11 directions used for this treatment. In order to reduce the likelihood of assignment errors in this process, a Python script was written to automate the selection process somewhat; each potential matchable feature in the experimental data (whether peak or coherence edge) was selected directly from the relevant data slice and the corresponding for the feature was recorded; these values were then used as sort parameters. This sort generated a list of the nearest theoretical dispersion surfaces in our set of [hkl] directions, and only surfaces that passed through the feature within 1 cm^{−1} (Δω) were considered as potential matches. Depending on the relative sharpness of the scattering feature, some features of less than 1 cm^{−1} were discarded as being insufficiently clear to match. Each sort then provided the dispersion curve label, the q point (in terms of fractional vector) and the mode number (using the mode identification in GULP) for use in model fitting, assuming that the Δω condition was met and the feature was sufficiently distinct in both theoretical and experimental data sets.
This process is clearly amenable to automated feature identification via a mathematical optimization formalism. However, for this initial work, the same process as is used for mode assignment in other spectroscopy has been used and only clearly distinct features have been selected for potential comparison to experimental data.
With these criteria, of the 31 identified features in 11 cuts through the LennardJonesderived data, only 20 could be unambiguously assigned to the experimental data. The labelling is provided in Fig. 8 for these 20 features, where the arrows are labelled with the relevant direction in q space. The upper values (black) refer to the experimental data and the lower values (red) to the model. To aid in the visualization of these points, Fig. S5 (in the supplementary text) shows how the sampling of (Q, ω) space has been accomplished, by projecting the points labelled in Fig. 8 onto the Q scale used for Figs. 3 and 6.
The final step in the analysis process involved fitting two of the models (LJ and Mei–Davenport) to these (q, ω) points using GULP's internal leastsquares minimization routine. In this procedure, the (q, ω) points were input as observables and the optimal parameters were obtained for both models from a variety of initial values to ensure that a reasonable global minimum was obtained. For the Mei–Davenport model, the EAM density terms were not fitted, although the was allowed to relax in one fit and fixed in the other to explore the effect of fixing the in such a model.
4.2. Results from the fitting of polyCINS data to two models for aluminium
The fitting process proved very successful for the case of the LennardJones potential model, and a global minimum was found with values of A and B of 28273.896 eV A^{−12} and 46.590 eV A^{−6}, respectively, keeping the constant fixed. The fitting process applied to the Mei–Davenport model, whilst successful, was considerably more methodologically dubious as the parameter space for the process is considerably larger and, as this work is not specifically targeted at producing a more physically accurate MEAM model, little effort was spent on ensuring that a true global empirical minimum was reached. However, as the EAM density parameters were kept fixed, i.e. were not included as fitting parameters, the fit resulted in changes to the E_{c}, α, β and γ parameters (with new values of 3.335, 4.57, 7.047 and 11.326 eV, respectively) in the EAM functional part of the potential, with φ_{0} and δ changing to 0.1330 and 7.3866 eV, respectively. The final parameterization of each model is presented in Table 3.

Thus, in Fig. 9, the initial and final (fitted) versions of the Mei–Davenport and LennardJones models were used to generate S_{coh}′(Q, ω) data sets equivalent to those found in Fig. 3, and constant Q cuts were taken through these data sets, following the process described in the previous section. The figure presents a representative example [for median Q = 4.6 Å^{−1}, with a cut width of 0.0667 Å^{−1} (median value ± 0.0334 Å^{−1})] of these data comparisons; more have been provided in the supplementary text. As can be seen, the key features being tracked are the peak corresponding to the [531] dispersion curve at 145 cm^{−1} (18.0 meV) and the coherence edge feature corresponding to the [422] dispersion curve at 200 cm^{−1} (24.8 meV) in the experimental data. Curves (a) and (c) show the theoretical S_{coh}′(Q, ω) generated from the initial versions of the models and clearly illustrate the better agreement with experiment provided by the LJ model. Curves (b) and (d) are the equivalent S_{coh}′(Q, ω) data generated after the fitting procedure It is clear that both models show significant improvement; in particular, the peak corresponding to the [531] direction shows much improved agreement with the experimental data. This is not surprising given that the features discussed were used as observables in the fitting process. However, selection of other cuts also produces features that are in better agreement with experiment (see supporting text for additional examples).
At this point in the analysis, it becomes clear that the present process lends itself very naturally to an iterative approach to the fitting process; although the present treatment deals with only a single `run through' of the method, the most sensible means of improving fits [and hence the quality of the model generating S_{coh}′(Q, ω)] would be to take the outputs of the current method and, rather than moving straight to bulk properties and dispersion curves, to reapply the process (probably several times) by taking cuts through the data set generated by the new model(s) and running through the feature identification and the fitting steps again. This approach, which would resemble a profile process as used for diffraction data (in effect, inelastic profile refinement), would minimize the differences between the theoretical and experimental S_{coh}′(Q, ω); work is in progress to demonstrate this approach.
Once the fitted models have been inspected for agreement with experiment, the final stage in the analysis is that of generating bulk properties and dispersion curves for the original and fitted models. Fig. 10 presents the dispersion curves for the two versions of the LennardJones and of the Mei–Davenport models compared with the singlecrystal dispersion curve data of Stedman & Nilsson. Rather encouragingly, both fitted potential models generate dispersion curves that are very similar, illustrating that the sampling of is consistent for both models. Both of the fitted models also produce dispersion curves that are in better agreement with the experimental curves, after allowing for the difference in temperature: the Stedman & Nilsson data were taken at 80 K, whereas the models generated are for data taken at 10 K. The higher temperatures will result in slightly softer modes and hence lower maximum frequencies at the zone boundaries. Of course, none of the models effectively reproduce the curvature of the TA modes in the [110] direction: both models have very short cutoff distances for the interactions (first nearest neighbour for the LJ model and fourth nearest neighbour for the Mei–Davenport model), which will significantly influence the curvature of the dispersion curves in this region. Indeed, the work by Gilat & Nicklow (1966) suggests that effective Born–von Karman force constant models in metals such as aluminium are sensitive to nearest neighbour interactions out to at least the eighth nearest neighbour distance. However, both models do show an improved agreement with experiment (both for the singlecrystal values and for the data reported in the present work).
Finally, the bulk properties of aluminium were calculated for both fitted models. The results are presented in Table 4. The fitted LennardJones model, which produces improved dispersion curves, nevertheless performs somewhat less well than the original model as far as the bulk properties are concerned. This is unsurprising given that the initial model was fitted to experimental elastic constants, but changes to the A and B are relatively small. The bulk property calculations for the Mei–Davenport model were handled in two ways; the first was a straight fixedlattice calculation where the potential generated very good agreement with experimental data; in the case of binding energy (not strictly valid for fixedlattice calculations), Young's and shear moduli, and elastic constant predictions, the fitted model outperforms the original model and generates predicted bulk properties consistently closer to experimental values. With the constraint of a fixed removed, the model fitted to the S_{coh}′(Q, ω) data produced a second set of predicted bulk properties (in parentheses in Table 4). Although this results in a relaxation of the giving rise to a constant that is significantly too large (4.17 Å, rather than the experimental value of 4.05 Å), the model performs much better than either the LennardJones (fitted) or the original Mei–Davenport model in terms of predicted binding energy and the other bulk properties, especially the elastic moduli (Young's, bulk and shear). We have demonstrated that the results can be markedly improved simply by expanding the cutoff of the LJ 12–6 model to 12.0 Å. This results in a model that provides broadly similar agreement (in terms of bulk values) to that of the original LJ model (fitted from elastic constants), yet requires no adjustment of the constants (i.e. the model predicts a spacing of 4.05 Å when allowed to relax). The resultant values of the parameters are included in Table 3 but further discussion is postponed.

4.3. Discussion on the extension of the method to other systems
As has been stated earlier, aluminium was chosen to illustrate the methodology for this work because it has the simplest possible crystalline structure as well as being a very well understood material in terms of both bulk properties and dynamics. Given the complexity of polycrystalline data sets, aluminium represents the simplest possible case to apply in terms of both basis size and symmetry, yet for this method to be generally useful, it should be extensible to materials with polyatomic basis sets and should also provide some demonstrable advantages to the current method of analysing powder spectra – namely the incoherent approximation.
Currently, the standard approach to assigning vibrational frequencies for polycrystalline coherent scattering systems is via the socalled incoherent approximation, a detailed treatment of which can be found elsewhere (Mitchell et al., 2005; Kearley, 1995). In this approach, the experimental data are integrated over the full angular range of detectors, which provides greatly improved statistics at the cost of obscuring all explicit Q dependence in the resulting twodimensional (frequency versus integrated intensity) data sets. The general method effectively treats the resulting data as a means of experimentally determining the phonon g(ω). These data are then compared, with minimal processing, with a gamma point calculation [typically using DFT and software such as PHONON or aCLIMAX (RamirezCuesta, 2004) to postprocess the force constant outputs into simulated inelastic neutron intensity data], and some implicit Q dependence is then inferred from relative intensities or the intensity profile as a whole. As an analysis method, it has much to recommend it: the method is very computationally efficient (a gamma point calculation is relatively computationally inexpensive and can be performed on a desktop workstation in very little time for smallunitcell systems) and, as has been mentioned, there are a number of freely available support software packages available to assist in this analysis. However, it is clear that there are several issues with this approach, the most significant being that explicit Q dependence of the vibrational modes is lost entirely; as one is dealing with the density of vibrational states, one may not track the curvature of individual modes. Indeed, before the computational resources became available for routine DFT calculations, much of the most detailed simulation and fitting used semiempirical models and carefully considered correction factors (Egelstaff & Poole, 1969) to properly weight the integrated intensities. The scattering data were plotted as a function of Q^{2} at a given angle, and the highQ data were extrapolated back to yield a gradient at small Q^{2}, where the actual data shows large fluctuations due to coherent terms. This would result in semiempirical force constant fits that could be very difficult to interpret and assign properly, given the sensitivity of the fits to the relative intensity profiles (Kearley, 1995).
After the advent of the easily accessible computational resources required to directly generate intensities using DFT, the emphasis shifted to using the aforementioned DFT direct simulation approach, typically compared with directly integrated g(ω). However, this approach directly integrates the scattering over observed values of Q at a given energy and assumes that the coherent scattering averages out. Our calculations show that there are significant differences between the actual obtained from GULP and the above quantity obtained from the GULP polyCINS output. The most notable one is that of intensity differences between the strict incoherent especially at low Q, where contributions from the coherent scattering in this region produce a `summed up over Q/angles' profile for the incoherent approximation that significantly deviates from the There are also issues associated with fitting an improved model: DFT calculations do not, in general, provide precise matches to INS data sets, and the scaling approach (Mitchell et al., 2005) used to assign modes unambiguously can obscure the quality of a given calculation. In any case, DFT outputs cannot be `fitted' to provide functional models for T > 0 K systems with ease. The polyCINS method does not suffer from this limitation (although DFT inputs can be used to provide an initial starting point for finite temperature calculations), as the Q dependence of individual modes can be identified and tracked, without resort to either complex correction factors or scaling of frequencies.
As the size of the basis set increases from the monatomic basis used for this work, other features in the scattering data will become relevant to discuss – most notably the scattering from optic modes (as aluminium is monatomic, it does not possess optic modes). Although this work has restricted itself to the discussion of the dynamics of the aluminium system, and by definition scattering profiles derived from acoustic modes, the authors have measured a number of polyatomic systems (with lower symmetries than cubic aluminium) using this approach, most notably graphite (Roach, 2006; Roach, Heuser et al., 2013; Roach, Parker et al., 2013), MgD_{2} (Buckley et al., 2013) and C_{60} (Roach, 2006; Roach, Heuser et al., 2013; Roach, Parker et al., 2013). In all these cases, optic modes generate the same coherence edge and peak features (they are still subject to the same selection condition as acoustic modes) and can be measured and identified, although these can be more difficult to distinguish than in the present case, requiring extremely long data collection runs on highintensity instruments to provide sufficiently high count rates to distinguish these features from noise. This is especially so in the case of very large systems and systems with relatively `flat' optic mode branches (such as C_{60}), which require correspondingly high resolution sampling in the calculation of the polyCINS intensities. Lowersymmetry systems also appear to pose no particular problem, providing the sampling of is sufficiently tight.
Finally, zone boundary effects can add to the variation of intensities, and one might speculate that this issue might affect the identification of edge and peak features where scattering close to the zone edge is very much more intense (see Fig. 4b and comments in §2.4); indeed, it is very likely that a number of the most intense features in Figs. 7 and 8 are due to the orientational averaging of this effect. This is, however, more likely to be an issue with samples with crystallites of highersymmetry materials (such as aluminium), as the path is very simple and these effects will superimpose in the orientational averaging much more obviously. With lowersymmetry crystallites, this would probably average out into a smoother intensity profile. However, it is important to check on this. Fig. S5 in the supplementary text provides a convenient method of checking for bias introduced as a result of this effect, as well as a means of checking other sampling bias (TA rather than LA, for instance, or zone centre versus zone edge). In the case of aluminium, and the sampling and feature selection for this work, it appears that the sampling is evenly split between zone edge and other regions. It is quite clear that some coherence edge features are more pronounced near the zone edges, but it is also clear (from Figs. 8 and S5) that scattering beyond these areas is sufficiently intense to identify these features away from the zone edge.
5. Conclusions
In the present paper we describe the structure of an extension to the GULP program, which calculates the polycrystalline coherent inelastic neutron scattering directly from a dynamical matrix for the crystal. This model for S_{coh}′(Q, ω) can be compared directly with experimental measurements made using an inelastic neutron spectrometer, either as a complete contour plot or in terms of profiles along observed loci in (Q, ω) space. The method has been applied to aluminium as a simple example of a crystalline material for which dispersion curve data are available; this provides definitive corroboration of the methodology. Three popular semiempirical models have been simulated, along with a simple model generated for the purpose of method checking. It was found that these models differ significantly from each other in terms of the dispersion curves and the bulk properties predicted by each. The best performing of these four models (the LennardJones and the Mei–Davenport) were then used to identify and analyse the polycrystalline coherent inelastic neutron scattering spectrum from a polycrystalline aluminium sample. Cuts were used through the data to identify dispersive features that were then used as fitting observables in a leastsquares fit of the model to the neutron data.
The method described, which relies on the analyst to identify scattering features in the neutron data that correspond to singlecrystal dispersion curves in a polycrystal, has proven to be effective in the simple case of aluminium. The strength of the method is that it does not require full sampling of (Q, ω) space – even along the locus of a cut through experimental data – to generate fitting observables. Rather it applies an understanding of the `rules' behind coherent to identify scattering features that coincide with dispersion curves in singlecrystal samples, and then uses these points in (Q, ω) space to generate individual q points for fitting using dynamics codes. Furthermore, although fits to experimental data can be improved with the addition of computationally calculated twophonon and multiphonon scattering contributions, dynamic Debye–Waller factor contributions, multiple scattering corrections, and other (instrumentspecific) contributions, none of these are necessary to identify the majority of onephonon edges in a polycrystalline sample. This in turn means that the computational costs for a given analysis are orders of magnitude less than would be required for a full calculation using a total scattering approach. As one increases the size of a given the computational expense of the full calculation rapidly becomes prohibitive and the required sampling of itself becomes a limiting factor; even simple systems with unit cells containing less than 20 or so atoms require significant computational resources for such calculations. Work is underway on the extension of this method to systems with larger unit cells. With regard to the complementarity of the polyCINS method with incoherent inelastic neutron scattering, it is worth pointing out that, for systems dominated by that are not suitable for isotope substitution with coherently scattering nuclei, the polyCINS method would provide little additional useful information and so mode assignment via would be the most efficient method to use. However, for those materials that can be readily isotope substituted to take advantage of one or more elements with isotopes with appreciable coherent cross sections, the polyCINS method could be used and the signal from the would be calculated and added to produce a composite S′(Q, ω). This plot would be used to identify features with no Q dependence and exclude them from the search for Qdependent scattering features. Mixed metal hydrides/deuterides would be an example of where polyCINS would provide a more complete experimental verification of a given model than via the incoherent approximation or incoherent alone.
Although this type of experimental measurement has not been much used in the past, it seems clear that, with the power of modern computational resources, it has the potential to become an important technique for analysing the dynamics of a wide range of intrinsically polycrystalline solids that have coherent cross sections (and GULP code, along with the analysis tools (written in Python) used to efficiently identify and compare dispersion curves and theoretical and experimental data sets.
can be simulated to isolate the coherent scattering features for systems with more mixed coherent–incoherent cross sections). In order that this approach be more accessible, the software used for this work will shortly be available in the next release of theSupporting information
Supplementary text. DOI: https://doi.org//10.1107/S0021889813023728/he5613sup1.pdf
Acknowledgements
The authors gratefully acknowledge the financial support of the UK Engineering and Physical Sciences Research Council (EPSRC award EP/G049130) in the preparation of this work. The authors would also like to acknowledge the assistance of H. GonzalezVelez of the Cloud Computing Competency Centre, NCI, Dublin, Eire, and M. T. Garba, IDEAS Research Institute, Robert Gordon University, Aberdeen, for computational collaboration on the parallelization of the Scatter code and associated tools, and S. F. Parker and R. Bewley of the ISIS facility, Oxon, for helpful discussions and provision of additional data related to this investigation. JDG thanks the Australian Research Council for funding through the Discovery Program, as well as both iVEC and NCI for the provision of computing. The authors would also like to thank the anonymous referees for their constructive and helpful criticism in the review stage of this work. The research materials supporting this publication can be accessed by contacting the corresponding author.
References
Born, M. & Huang, K. (1956). Dynamical Theory of Crystal Lattices. Oxford University Press.
Buckley, A., Roach, D. L., Garba, M. T., Buckley, C. E., Ross, D. K., Gale, J. D., Sheppard, D. A., Carter, D. J. & Taylor, J. W. (2013). In preparation.
Budi, A., Henry, D. J., Gale, J. D. & Yarovsky, I. (2009). J. Phys. Condens. Matter, 21, 144206. Web of Science CrossRef PubMed
Clark, S. J., Segall, M. D., Pickard, C. J., Hasnip, P. J., Probert, M. J., Refson, K. & Payne, M. C. (2005). Z. Kristallogr. 220, 567–570. Web of Science CrossRef CAS
Cleri, F. & Rosato, V. (1993). Phys. Rev. B, 48, 22–33. CrossRef CAS Web of Science
Daw, M. & Baskes, M. (1983). Phys. Rev. Lett. 50, 1285–1288. CrossRef CAS Web of Science
Egelstaff, P. A. & Poole, M. J. (1969). Experimental Neutron Thermalisation. Oxford: Pergamon Press.
Gale, J. D. & Rohl, A. L. (2003). Mol. Simul. 29, 291–341. Web of Science CrossRef CAS
Gilat, G. & Nicklow, R. (1966). Phys. Rev. 143, 487–494. CrossRef CAS Web of Science
Hafner, J. & Schmuck, P. (1974). Phys. Rev. B, 9, 4138–4150. CrossRef CAS Web of Science
Halicioǧlu, T. & Pound, G. M. (1975). Phys. Status Solidi, 30, 619–623.
Jasper, A. W., Schultz, N. E. & Truhlar, D. G. (2005). J. Phys. Chem. B, 109, 3915–3920. Web of Science CrossRef PubMed CAS
Kang, J. K., Lee, J. Y., Muller, R. P. & Goddard, W. A. (2004). J. Chem. Phys. 121, 10623–10633. Web of Science CrossRef PubMed CAS
Kearley, G. (1995). Nucl. Instrum. Methods Phys. Res. Sect. A, 354, 53–58. CrossRef CAS Web of Science
Lefmann, K. & Nielsen, K. (1999). Neutron News, 10(3), 20–23. CrossRef
LennardJones, J. E. & Ingham, A. E. (1925). Proc. R. Soc. London Ser. A, 107, 636–653.
Mei, J. & Davenport, J. (1992). Phys. Rev. B, 46, 21–25. CrossRef CAS Web of Science
Mishin, Y., Farkas, D., Mehl, M. & Papaconstantopoulos, D. (1999). Phys. Rev. B, 59, 3393–3407. Web of Science CrossRef CAS
Mitchell, P. C. H., Parker, S. F., RamirezCuesta, A. J. & Tomkinson, J. (2005). Vibrational Spectroscopy with Neutrons. Singapore: World Scientific.
Nye, J. F. (1957). Physical Properties of Crystals. Oxford University Press.
Pham, H. H., Williams, M. E., Mahaffey, P., Radovic, M., Arroyave, R. & Cagin, T. (2011). Phys. Rev. B, 84, 064101. Web of Science CrossRef
RamirezCuesta, A. J. (2004). Comput. Phys. Commun. 157, 226–238. CAS
Roach, D. L. (2006). PhD thesis, University of Salford, Greater Manchester, UK.
Roach, D. L., Gale, J. D. & Ross, D. K. (2007). Neutron News, 18(3), 21–23. CrossRef
Roach, D. L., Heuser, B., Ross, D. K., Garba, M. T., Baldissin, G., Gale, J. D. & Abernathy, D. L. (2013). In preparation.
Roach, D. L., Parker, S. F., Ross, D. K., GonzalezVelez, H., Garba, M. T., Gale, J. D., Russina, M., Granroth, G. E. & Bewley, R. I. (2013). In preparation.
Ross, D. K. (1973). J. Phys. C, 6, 3525–3535. CrossRef CAS Web of Science
SanchezPortal, D., Artacho, E. & Soler, J. M. (1995). Solid State Commun. 95, 685–690. CAS
Schuth, F., Bogdanovic, B. & Felderhoff, M. (2004). Chem. Commun. pp. 2249–2258.
Sheng, H. W., Kramer, M. J., Cadien, A., Fujita, T. & Chen, M. W. (2011). Phys. Rev. B, 83, 134118. Web of Science CrossRef
Squires, G. L. (1978). Introduction to the Theory of Thermal Neutron Scattering. Cambridge University Press.
Stedman, R. & Nilsson, G. (1966). Phys. Rev. 162, 549–557. CrossRef Web of Science
Streitz, F. & Mintmire, J. (1994). Phys. Rev. B, 50, 11996–12003. CrossRef CAS Web of Science
Sutton, A. P. & Chen, J. (1990). Philos. Mag. Lett. 61, 139–146. CrossRef Web of Science
Tang, X., Li, C. W. & Fultz, B. (2010). Phys. Rev. B, 82, 184301. Web of Science CrossRef
Taylor, A. D., Arai, M., Bennington, S. M., Bowden, Z. A., Osborn, R., Andersen, K., Stirling, W. G., Nakane, T., Yamada, K. & Welz, D. (1991). Proceedings of the 11th Meeting of the International Collaboration on Advanced Neutron Sources. KEK Report 90–25. Tsukuba, Japan.
Turchin, V. F. (1965). Slow Neutrons. Jerusalem: IPST.
Van Hove, L. (1954). Phys. Rev. 95, 249–262. CrossRef CAS Web of Science
Willendrup, P., Farhi, E. & Lefmann, K. (2004). Physica B, 350, E735–E737. Web of Science CrossRef CAS
This is an openaccess article distributed under the terms of the Creative Commons Attribution (CCBY) Licence, which permits unrestricted use, distribution, and reproduction in any medium, provided the original authors and source are cited.